ENVIRONMENTAL EFFECTS ON COMPOSITES FOR AIRCRAFT ENVIRONMENTAL EFFECTS ON COMPOSITES FOR AIRCRAFT...
Embed Size (px)
Transcript of ENVIRONMENTAL EFFECTS ON COMPOSITES FOR AIRCRAFT ENVIRONMENTAL EFFECTS ON COMPOSITES FOR AIRCRAFT...
ENVIRONMENTAL EFFECTS ON COMPOSITES FOR AIRCRAFT
Richard A. Pride NASA Langley Research Center
The influence of the operational environment on the behavior of composite materials and aircraft components fabricated with these composite materials is a subject of continuing concern both for the aircraft manufacturer and the air- line operator. The structural weight savings and the potential for manufactur- ing cost savings have been well documented in a number of composite hardware development programs in recent years. These advantages have left the question of long-term environmental durability for composites as the major undetermined issue for widespread acceptance and application.
This paper reports on the interim results from a number of ongoing, long- term, environmental effects programs. The flight service experience to date of composite components is evaluated. In addition, the influence of a number of worldwide, ground-based outdoor exposures on the physical and mechanical proper- ties of six composite materials is discussed. In particular, the current extent of the ultraviolet surface degradation and the moisture gained by diffusion is shown, Finally, several new environmental programs which have been started recently are reported to show the type of information that can be expected to be available in the next few years.
FLIGHT SERVICE OF COMPOSITE COMPONENTS
A number of composite structural components have been designed, manufac- tured, tested, and placed in operational service on a variety of aircraft. This operational flight service is monitored periodically to evaluate the long- term experience with composite durability. The types of aircraft and composite components are shown in figure 1. The L-1011 application is six fuselage fair- ing panels involving two types of Kevlar-49 epoxy composite on each of three airplanes (ref. 1). Three graphite-epoxy material systems are used for the spoilers on 27 Boeing 737 airplanes (ref. 2). A fourth graphite-epoxy material is used in the upper, aft rudder segment on ten DC-10 airplanes (ref. 3), and boron-aluminum composite skin is used in a panel on the aft pylon adjacent to the engine on three DC-10 airplanes (ref. 4). Boron-epoxy is used as a selective reinforcement in the aluminum aft fuselage, or tail cone, of an Army CH-54B helicopter (ref. 5) and in the aluminum center wing box of two Air Force C-130 transports (ref. 6).
The status of these composite structural components in the Langley flight service program, as of January 1, 1978, is given in table I. The boron-epoxy composite in the CH-54B helicopter tail cone has been in service for the longest calendar time, six years, but it has been flown very little compared to the other types of aircraft. The Kevlar-49 epoxy in the L-1011 fairing panels has
accumulated the greatest single component flight time, 13 138 flight hours in five years of service. The graphite-epoxy in the 108 spoilers on the 737 air- planes has accumulated the greatest total component flight hours, 921 600 in four and one-half years. The graphite-epoxy in one of the DC-10 upper aft rudders has been acquiring flight service time at the.greatest rate of any of the components in the table, a rate of 400 hours per month or about 13 hours per day. Overall the 142 composite components have accumulated in excess of one million component flight hours in service around the world with 17 operators. Each of these composite components has been inspected at least annually by the manufacturer, under terms of the NASA contracts. There have been no significant incidents or damage detected in any of these flight components. Maintenance has been reported as less than that required on similar standard, production parts.
The large number (108) of replicate spoilers with graphite-epoxy skins allows a program of planned retrievals from flight service without seriously impairing the total exposure. Six spoilers are selected at random for removal annually, two of each of the three material systems. These spoilers are shipped to The Boeing Company where they are nondestructively inspected by ultrasonic C-scan. The C-scan record is compared with similar records made at the comple- tion of manufacturing. To date, no significant differences have been observed. Three of the six spoilers are then selected for destructive testing and the remaining three are returned to flight service.
For destructive testing the spoilers are mounted in the same static test jig as was used for the initial airworthiness certification tests (ref. 2). A distributed load is applied to the outer surface of the spoiler, simulating aerodynamic loads, and the magnitude is increased until failure occurs. Results of these residual static strength tests on the graphite-epoxy spoilers are shown in figure 2. The residual strengths for each material system have been divided by the failure strength o.f the initial certification test for each material, and the results are presented nondimensionally as a function of the time in service. A scatter band for strength tests of 16 new replicate spoilers manu- factured with the T300-5209 graphite-epoxy material has been superimposed on the individual tests of spoilers removed from service. In four years of service, the scatter in strength for the individual spoilers generally falls within the width of the new spoiler strength scatter band; an indication of essentially no degradation in strength.
After several years of unsuccessfully attempting to determine the moisture absorbed by the graphite-epoxy spoilers in service, a technique of cutting plugs from near the trailing edge was developed (fig. 3). The eight rectangular areas shown with an arrow in the center of each represent the whiffletree load- ing areas for static strength tests. Since failures always have initiated near the leading edge at one of the center hinges, it has been determined that three plugs of 6.4 cm (2.5 in.) diameter could be cut from the region behind the loading areas without influencing the failure load. These plugs, which consist of aluminum honeycomb core, two graphite-epoxy face sheets, two layers of epoxy film adhesive and two exterior coats of polyurethane paint, have about
90 percent of their weight in the composite faces, including the paint and adhesive. A good determination of the moisture level in the spoiler can be made by drying the plug and noting the weight change. After three years of service with Lufthansa Airlines in Germany, p lugs taken from a T300-5209 graphite-epoxy spoiler indicated a moisture content of 0.64 percent, based on the composite weight. Somewhat greater significance may be attached to this value when corrections have been determined for relative differences in equilibrium moisture levels in the paint, the composite matrix, and the adhesive.
Subsequent to the introduction into flight service of the graphite-epoxy- skinned spoilers, a development program was undertaken for an all-composite spoiler which included glass-epoxy honeycomb core, molded graphite-epoxy hinge fittings and leading edge spar, and thermoplastic graphite-polysulfone skins (ref. 7). It was recognized that the polysulfone matrix had an environmental sensitivity to phosphate-ester-based hydraulic fluids, and the laboratory test- ing demonstrated this in elevated temperature, stressed immersions. However, based on the room temperature experience it was believed that the material could be successfully used in flight components with only minor, intermittent exposures to hydraulic fluid leakage from the spoiler actuators. Twelve of these spoilers were fabricated and placed in service on six of the aircraft that were flying graphite-epoxy spoilers. After six months of operational flight service the two spoilers installed on Aloha Airlines were reported to have developed significant delamination of the lower surface skin directly aft of the actuator attachment fitting (fig. 4). Within a month a third spoiler was reported as starting to experience delamination, so it was decided to remove all the remaining graphite-polysulfone spoilers. A closeup view of the delaminated area is shown in the photograph in figure 5. This experi- ence demonstrated the difficulty of performing adequate laboratory accelerated environmental testing and provided a good example of the necessity for flight service evaluation.
There have been several instances in which the graphite-epoxy spoilers have received damage in service sufficient to require repairs. Examples of these are illustrated in figure 6. On this program, damaged spoilers are removed from the aircraft and returned to The Boeing Company for repair. Repairs are made by cutting out the damaged area, replacing honeycomb core as needed, and replacing graphite-epoxy plies on a one-for-one basis with each ply lapped over the underlying one by about 6 mm (0.25 in.). One piece of adhesive film is placed under the patch assembly and the built-up patch is cured and bonded in one cycle in an autoclave with the spoiler supported in its original assembly tooling (ref. 7). The repaired spoiler is ultrasonically inspected and returned to flight service with the airline which had previously used it.
WORLDWIDE GROUND-BASED OUTDOOR EXPOSURE
As a parallel part of the flight service exposures of composite components, a number of replicate mechanical property specimens have been manufactured from the same composite material systems used in the components. These speci- mens have been mounted in racks which are deployed on roo